Do you need custom fasteners created with Alloy 60? Since our inception, Elgin Fastener Group has met every challenge of providing Quality, Timely, Cost-effective solutions for specialty fastener applications. Every product is built to your specifications, using your prints if necessary.
Below are the technical specifications of the Alloy 60 Bar Stock we have available to meet your needs.
Special Metals INCONEL® Alloy 600
Subcategory: Metal; Nickel Base; Superalloy Key Words: Inconel 600, ASTM B163, ASTM B166, ASTM B167, ASTM B168, ASTM B366, ASTM B516, ASTM B517, ASTM B564, ASTM B751, ASME SB-163, SB-166 – SB-168, SB-564, Boiler Code Sections I, III, VIII, IX, Nickel-Chromium Alloy, NACE MR-01-75; QQ-W-390; MIL-R-5031, MIL-T-23227, MIL-N-23228, MIL-N-23229; AFNOR NC 15 Fe, SAE AMS 5540, 5580, 5665, 5687, 7232; DIN 17742, 17750 – 17754; Werkstoff Nr. 2.4816; VdTUV 305, UNS N06600; BS 3072 – 3076 (NA14)
|Cr||14 – 17|
|Fe||6 – 10|
Material Notes: Nickel content above includes cobalt. A nickel-chromium alloy with good oxidation resistance at high temperatures and resistance to chloride-ion stress-corrosion cracking, corrosion by high-purity water, and caustic corrosion. Used for furnace components, in chemical and food processing, in nuclear engineering, and for sparking electrodes. Standard product forms are round, hexagon, extruded section, flats, forging stock, pipe, tube, plate, sheet, strip, and wire.
Data provided by the manufacturer, Special Metals.
MicroGroup’s inventory of small diameter 304 and 316 and other stainless steel, nickel based alloys, and titanium alloys exceeds 5 million feet. Redraw of material to specific sizes and shapes, as well as secondary operations to convert tubing into components and assemblies. Visit http://www.microgroup.com or Phone 1-800-ALL-TUBE (1-800 255-8823) or 1-508-533-4925.
|Density||8.47 g/cc||0.306 lb/in³|
|Tensile Strength, Ultimate||655 MPa||95000 psi||Annealed. Value at room temperature. Value at 550°C is 550 MPa.|
|Tensile Strength, Yield||310 MPa||45000 psi||Annealed. Value at room temperature; 0.2% offset. Value at 550°C is 180 MPa.|
|Elongation at Break||45 %||45 %||Annealed. Value at room temperature. Value at 550°C is 42%.|
|Electrical Resistivity||0.000103 ohm-cm||0.000103 ohm-cm|
|Magnetic Permeability||1.01||1.01||at 200 oersted (15.9 kA/m)|
|Curie Temperature||-194 °C||-317 °F|
|CTE, linear 20°C||13.3 µm/m-°C||7.39 µin/in-°F||20-100°C|
|Heat Capacity||0.444 J/g-°C||0.106 BTU/lb-°F|
|Thermal Conductivity||14.9 W/m-K||103 BTU-in/hr-ft²-°F|
|Melting Point||1354 – 1413 °C||2470 – 2580 °F|
|Solidus||1354 °C||2470 °F|
|Liquidus||1413 °C||2580 °F|